U.S. Department of Transportation
Federal Highway Administration
1200 New Jersey Avenue, SE
Washington, DC 20590
2023664000
Federal Highway Administration Research and Technology
Coordinating, Developing, and Delivering Highway Transportation Innovations
This report is an archived publication and may contain dated technical, contact, and link information 

Publication Number: FHWAHRT04097
Date: August 2007 

Measured Variability Of Southern Yellow Pine  Manual for LSDYNA Wood Material Model 143PDF Version (2.92 MB)
PDF files can be viewed with the Acrobat® Reader® 1.8 RATE EFFECTSA number of approaches are available to accommodate strainrate sensitivity. Simple approaches scale the input strengths or moduli as a function of strain rate. More sophisticated approaches use viscoplastic mechanisms. Viscoplastic mechanisms retard the development of plasticity, which allows the stress state to exceed the static failure surface. Viscoplastic mechanisms also increase the stiffness in conjunction with strength if plastic hardening is modeled in the prepeak regime. Both types of formulations are easy to implement and are computationally efficient. Therefore, two methods are implemented. One method scales each strength as a function of strain rate, effectively expanding the failure surface. The second method is viscoplastic. Both methods are discussed here. However, the shifted surface method is the easiest to fit, and it is the only method that has been validated to date, so it is the only active option in the wood model at this time. 1.8.1 High StrainRate DataA common test for measuring strainrate effects is the split Hopkinson pressure bar (SHPB). Hopkinson bar data for pine are shown in figure 19.^{(11)} Here, the dynamictostatic stress ratio is plotted as a function of impact velocity for both the parallel and perpendicular directions. Rate effects are more pronounced in the perpendicular direction than in the parallel direction. Also plotted in figure 19 are theoretical curves derived from shock theory (i.e., conservation of mass and momentum across a shock front). The theoretical stress enhancement factors are: where: Â = ratio of dynamictostatic stress r = average wood density rs = wood solid phase density a = empirical shape factor for the stressstrain curve Values of rs = 1500 kilograms per square meter (kg/m^{2}) and a = 1.35 are reported by Reid and Peng^{(11)} for wood and pine. For southern yellow pine with a density of r = 530 kg/m^{2} at 12percent moisture content, the stress enhancement curves reduce to: where V is measured in m/s. These curves indicate that the stress enhancement in the perpendicular direction is much greater than that in the parallel direction. However, the curves tend to underestimate the stress enhancement, particularly at lowimpact velocities (see figure 19). To fit the rateeffect model parameters, the stress enhancement ratios need to be derived as a function of strain rate. To do this, impact velocity must be converted to strain rate. However, Reid and Peng^{(11)} did not report this conversion. Figure 19. Hopkinson bar tests indicate that the measured strength of pine increases with impact velocity. Source: Pergamon, Elsevier Science Ltd.^{(11)} Bragov and Lomunov also measured the dynamic properties of pine using the SHPB technique.^{(23)} Stressstrain diagrams are depicted in figure 20. Data are measured parallel and perpendicular to the grain. In addition, two curve sets are shown for each direction, which correspond to two strain rates (approximately 1000 per second(s^{1}) and 500 s^{1}). The data indicate that both strength and parallel stiffness increase with strain rate. Figure 20. Hopkinson bar data indicate that strength and stiffness increase with strain rate. Source: EDP Sciences.^{(23)} Parallel and perpendicular strength ratios versus strain rate are needed to fit the rateeffect model. Here, those ratios are estimated. Bragov and Lomunov report a static parallel compressive strength of X_{C} = 41.4 MPa for pine.^{(23)} This strength is used to calculate the parallel strength ratios from figure 20. Calculated values are Â(0°) = 2.3 at 1000 per second (s) and Â(0°) = 1.7 at 500/s. Bragov and Lomunov did not report a static perpendicular compressive strength for Y_{C}.^{(23)} Therefore, one cannot directly estimate the perpendicular strength ratio from figure 20. Instead, the Reid and Peng velocitystrength ratio relationships in equation 76 are used to estimate the impact velocities and perpendicular strength ratios.^{(11)} Impact velocities of 262 m/s and 192 m/s are derived from the parallel relationship in equation 76 for Â(0°) = 2.3 and Â(0°) = 1.7, respectively. Using these velocities, perpendicular strength ratios of Â(0°) = 9.0 and Â(0°) = 5.3 are derived from the perpendicular relationship in equation 76. These ratios are reported in table 11.
1.8.2 Shifted Surface Model TheorySeparate rateeffect formulations are modeled for the parallel and perpendicular modes because the Reid and Peng data indicate that dynamic strength enhancement is more pronounced in the perpendicular direction than in the parallel direction.^{(11)} The rateeffect formulations increase strength with increasing strain rate by expanding each yield surface: Parallel Perpendicular
Excess stress components depend on the value of the fluidity parameter, h; the stiffness, C; and the effective strain rate, . When rate effects are requested via the flag IRATE = 1, dynamic strengths are used in place of the static strengths in the yield surface formulations (in equations 13 and 14, or in equations 44 and 45). Four effective fluidity parameters are used (h_{}, h_{c}, h_{^}, and h_{c^}). Two parameters are needed for the parallel modes―one for the tensile and shear strengths, and a second for the compressive strength. Two parameters are also needed for the perpendicular modes. Each effective fluidity parameter is formulated from two input parameters: The twoparameter formulation allows the user to model a nonlinear variation in dynamic strength with strain rate.^{(24)} Setting n_{} = 0 or n_{^} = 0 allows the user to model a linear variation in dynamic strength with strain rate. The total number of input parameters is six. Three parameters are input for the parallel modes (h_{}, h_{c}, and n_{}) and three parameters are input for the perpendicular modes (h_{}, h_{c}, and n_{^)}. Singleelement simulations performed with and without rate effects (500/s) are shown in figure 21 for roomtemperature clear wood at 12percent moisture content. The dynamictostatic strength ratio Â(0°) = 1.7, previously listed in table 11, was used to set the rateeffect parameters for the compressive simulation. These parameters are given in table 12. The plots in figure 21 indicate that different dynamictostatic strength ratios naturally occur for the tension simulations than for the compressive simulations, even though h_{} = h_{c}. This is because the tensile and compressive simulations have the same excess stress components, but different static strengths. Figure 21. These singleelement simulations demonstrate the rateeffect behavior of the shifted surface formulation at 500/s.
1.8.3 Viscoplastic Model TheoryViscoplastic algorithms allow the stress state to exceed the yield surface. The excess stress depends on the value of the fluidity parameter, h; the stiffness; and the strain rate. The viscoplastic (dynamic) stresses attained in uniaxial simulations are approximately those given in equations 77 through 82. Single and twoparameter viscoplastic formulations are available. The singleparameter formulation was developed by Duvaut and Lions and models a linear variation in strength ratio with strain rate.^{(25)} This is accomplished by specifying a constant value for each fluidity parameter (independent of strain rate). However, a linear variation is not necessarily appropriate for wood, as demonstrated in figure 19. A twoparameter formulation was recently suggested by Murray to model a nonlinear variation in strength ratio with strain rate.^{(24)} The twoparameter formulation was previously given in equations 83 through 86. The viscoplastic formulation uses the same input parameters as the shifted surface formulation. The behavior of the viscoplastic model is shown in figure 22 for h = 0.0000094 s and four values of n. Here, the strength enhancement ratio (dynamictostatic) has been plotted as a function of the strain rate. The smaller the value of n, the greater the strength enhancement at a given strain rate. The behavior of the twoparameter formulation reduces to that of the singleparameter formulation for n = 0. Thus, the DuvautLions singleparameter model is a subset of the twoparameter model. Figure 22. Twoparameter viscoplastic model is flexible in fitting data. The twoparameter viscoplastic update scheme is implemented as follows:
At each time step, and are calculated and saved by the plasticity algorithm. Then, equations 87 through 91 are applied to update the viscous solution. The inviscid and instantaneous elastic solutions are obtained as limiting cases of the implementation. This algorithm is easy to implement because the plasticity algorithm is not modified. The viscoplastic formulation is separate from and follows the plasticity algorithm. Separate formulations are implemented for the parallel (s_{11}, s_{12}, and s_{13}) and perpendicular modes (s_{22}, s_{33}, and s_{23}), because the Reid and Peng test data suggest that the rate effects depend on grain orientation.^{(11)} The parallel stress components are updated with the parallel fluidity parameters, while the perpendicular stress components are updated with the perpendicular fluidity parameters. At this time, viscoplastic implementation requires only four parameters as input. These are h_{} = h_{c} and n_{} for the parallel modes, and h_{^} = h_{c^} and n_{^} for the perpendicular modes. Therefore, one cannot specify separate dynamic overstresses for the tensile and compressive modes. Enhancement from four to six parameters could be conducted at a later date. Singleelement simulations performed with and without viscoplastic rate effects (500/s) are shown in figure 23 for roomtemperature clear wood pine at 12percent moisture content, using the input parameters specified in table 12.^{5} The primary difference between the viscoplastic simulations and the shifted surface simulations (figure 21) is that the viscoplastic tensile simulation is nonlinear to peak, whereas the shifted surface simulation is linear. This is because plastic strains are being calculated with the viscoplastic formulation, not the shifted surface formulation. The user has no control over the linearity or nonlinearity with either formulation. Also note that the compressive simulations calculated with viscoplasticity attain the same dynamic peaks as those calculated with the shifted surface formulation. Different hardening parameters were used in each simulation, so the hardening is not identical. On the other hand, the tensile simulations calculated with the viscoplastic formulation attain lower peak strengths than those calculated with the shifted surface formulation. This is because damage accumulates in tension (not compression) and is applied to the stresses at the same time as viscoplasticity. Damage does not accumulate in tension during application of the shifted surface formulation. ^{5} Default hardening and softening parameters were not finalized at the time that these plots were made, so these figures cannot be reproduced using the current default material property values. 1.8.4 Default RateEffect ParametersDefault rateeffect parameters for the shifted surface formulation were previously given in table 12. They provide the strength enhancement ratios listed in table 11. No rateeffect data are available for Douglas fir, so the model uses the same default parameters as southern yellow pine. The viscoplastic algorithm uses four of the six shifted surface parameters (the compressive fluidity parameters are ignored). Figure 23. These singleelement simulations demonstrate the rateeffect behavior of the viscoplastic formulation at 500/s. 
Topics: research, safety, infrastructure, structures, materials Keywords: research, safety, infrastructure, structures, materials, wood, LSDYNA, orthotropic, material model, damage, rate effects, guardrail TRT Terms: guardrails, wood Updated: 04/12/2012
